OPEN Impact of n,γ-irradiation on organic complexes of rare earth metals Tatyana V. Balashova1, Sergey V. Obolensky2, Alexey N. Trufanov3, Mikhail N. Ivin2,3, Vasily A. Ilichev1, Andrey A. Kukinov1,2, Eugeny V. Baranov1, Georgy K. Fukin1 & 1,2 Received: 19 March 2019 Mikhail N. Bochkarev Accepted: 22 July 2019 The complexes of La, Ce, Nd, Sm, Eu, Tb and Yb with benzoxazolyl-phenolate, benzothiazolyl- Published: xx xx xxxx phenolate, benzoxazolyl-naphtholate, benzothiazolyl-naphtholate and 4,4,4-trifuoro-1-(2-thienyl)- 1,3-butanedione ligands were treated with n,γ-irradiation upon a sustained (45 h, absorbed dose of 120 krad, fux of neutrons 5·1013 n/cm2) and a pulse mode (3 ms, absorbed dose of 130 krad, fux of neutrons 3.6·1013 n/cm2). It was found that main characteristics of the compounds (shape of substance, color, IR absorption and photoluminescent spectra) have not changed. With an example of cerium
complex [Ce(OON)3]2 it was revealed that the molecular structure of compounds after strong pulse irradiation also does not changed. However, computer simulations of neutron exposure on the same complexes showed signifcant shift of metal atoms and ligands. Possible reasons for the detected discrepancy between experimental and calculated data are discussed.
Many organic complexes of lanthanides, due to the peculiarities of the electronic structure of the metal atom, possess luminescent and photovoltaic properties, which determine their use in modern optoelectronic devices and in biomedicine1. All methods and technologies where rare earth metal complexes are used assume their work under “normal” conditions, i.e. in the absence of specifc forms of exposure. However, over the past century, in the sphere of human activity, new areas have emerged and are rapidly expanding, where a new component — ionizing irradiation (InI) — is being added to ordinary conditions. Such areas include space, active zones of nuclear power plants, concentrating and processing radioactive materials enterprises, radio- therapy and diagnostics, territories polluted with nuclides as a result of accidents. Unfortunately, it is impossible to exclude the existing probability of contamination of the area by nuclides due to the explosion of nuclear warheads. Currently, in devices designed to operate under InI conditions, only inorganic semiconductor materials are used, although studies have shown their relatively low radiation resistance2–5. Tere are as well two papers on the radiation resistance of organic semiconductors in which the polymer/fullerene systems are considered as promising for designing solar cells operating under radiation conditions6,7. Metal-organic substances, as an alternative to inorganic analogues, have not been previously considered, despite the fact that in many respects (fexibility, weight, tunability of various characteristics, cost, processability) the latter are signifcantly inferior to organic derivatives. Te main reason for this situation was, apparently, the a priori prevailing opinion about the low radiation resistance of metal-organic compounds. Te conclusion was based on a comparison of the thermal, chemical, and photolytic stability of both types of substances. As far as we know, no special studies have been carried out on the radiation resistance of organic complexes. However, recently published data on the radioluminescent properties of aryl carboxylates of non-transition8,9, d-transition metals10 and lanthanides11 indirectly indicate that substances of this class may have sufciently high radiation resistance. In this paper, we report on the study of the efects of n,γ-radiation on lanthanide organic complexes in order to determine the possibility of their use in devices operating under conditions of enhanced radiation. As objects, we selected complexes with substituted phenolate and naphtholate ligands, the main physico-chemical charac- teristics and molecular structure of which were described by us earlier12–14. A modifed well-known europium 2-thenoyltrifuoroacetonate Eu(TTA)3(DME)2, which has a diferent type of ligands and has good luminescent properties, was also used.
1G. A. Razuvaev Institute of Organometallic Chemistry of Russian Academy of Sciences, Tropinina 49, 603950, Nizhny Novgorod, Russian Federation. 2Nizhny Novgorod State University, Gagarina avenue 23/2, 603950, Nizhny Novgorod, Russian Federation. 3Branch of RFYaTs-VNIIEF «Yu.E. Sedakov FNCP NIIIS», Tropinina 47, 603950, Nizhny Novgorod, Russian Federation. Correspondence and requests for materials should be addressed to M.N.B. (email: [email protected])
Scientific Reports | (2019) 9:13314 | https://doi.org/10.1038/s41598-019-49962-9 1 www.nature.com/scientificreports/ www.nature.com/scientificreports
Figure 1. Photo of the samples of the compounds [La(NpSON)3]2 (2), [Sm(NpSON)3]2 (3) and the glass tubes (1) before (right sample) and afer (lef sample) irradiation.
Results and Discussions All the complexes chosen for the study are quite stable in an inert atmosphere and in vacuum but hydrolyze slowly in air except the air-stable Eu compound. Upon heating they decompose above 180°С. Te compounds [Nd(NpSON)3]2, [Sm(OON)3]2, Eu(TTA)3(DME)2, [Tb(OON)3]2 and [Yb(NpSON)3]2 when excited by UV light generate intense metal-centered emission. Cerium complex shows only the ligand luminescence. For some com- 12 pounds, including [Ce(OON)3]2, the molecular structure has been determined by X-ray difraction method . Te listed properties, which are convenient for the identifcation of compounds, stipulated our choice of these substances as models for studying the radiation stability of metal-organic complexes. Te samples were processed by radiation generated upon the decay of 235U nuclei. Te full spectrum of radi- ation was used including α, ß, γ components and neutrons. However, since α and ß-components were fltered almost completely upon passage through the walls of the glass tubes, the material was exposed only by neutrons and γ-radiation. Te study included three stages: the frst two were carried out in a sustained mode (45 h), the third stage was pulse irradiation (3 ms). Te dose of absorbed radiation, with the neutron fux of 6·1012, 5·1013 and 3.6·1013 n/cm2, was 12, 120 and 130 krad, respectively. Afer irradiation, the color and appearance of the samples remained almost unchanged (Fig. 1). Since the color of the glass tube afer pulse irradiation changed (control sample 1), the complexes were overloaded into a new tube before photographing. Comparison of the IR spectra of the irradiated samples of the [La(NpSON)3]2, [Sm(OON)3]2, and Eu(TTA)3(DME)2 complexes with the spectra of the corresponding samples that were not processed did not reveal diferences (Fig. S1). Te set and intensity of the bands in the photoluminescence spectra of irradiated and non-irradiated solid samples of the same compounds also displayed no diference (Fig. 2). Te open-circuit voltage (0.3 V), short current (22 μA/cm2) and fll factor (15%) of the photovoltaic cell based on the irradiated sample of the ytterbium complex [Yb(NpSON)3]2 coincided with the corresponding character- istics of the cell containing the non-irradiated compound. It should be noted that the semiconductor properties of such widely used inorganic materials as Si, SiN, GaAs are changed signifcantly and irreversibly already when irradiated with an energy of 200 keV and an absorbed dose of 905 Gy (90.5 krad)2. Te crystals of the [Ce(OON)3]2 complex even afer intense pulse irradiation retained their shape, which made it possible to use X-ray difraction analysis to determine their molecular structure. Note that the study of the degradation of organic and metal-organic compounds under the action of InI at the molecular level has not previ- ously been carried out. Te analysis data showed that the structure of the treated complex is very slightly diferent from the structure of the compound which was not irradiated and the complex studied six years ago12. Diferences are manifested in a negligible change in the position of the ligands (Tables S1 and S2). Te greatest displacement of 0.482 Å is observed for C atoms of phenyl groups of terminal ligands. In Fig. 3 the molecular structure of irra- diated and non-irradiated [Ce(OON)3]2 complex are shown. For convenience of comparison, both structures are superimposed on one another in such a way that the metal atoms and the bridging oxygen atoms are superposed. Te data obtained gave grounds to suggest that n,γ-irradiation caused some changes in the molecular struc- ture of the studied complex. To test the assumption we compared the unit cell parameters of the irradiated com- 15 12 pound with those of the earlier obtained related complexes [Pr(OON)3]2 , [Eu(OON)3]2 and [Gd(OON)3]2 , which were not exposed to InI, and found that these parameters exactly correspond to the values of irradiated [Ce(OON)3]2. Tis prompted us to repeat the synthesis of the Ce complex and examine again its structure. Te cell parameters of the newly synthesized compound coincided with the parameters of the irradiated sample. Tus, the data obtained showed that (i) InI has not destroyed the crystal and molecular structure of the treated complex and (ii) the synthesis of organo-lanthanide complexes can give products with the same arrangement but with a diferent structure, even under the same preparation conditions. Te fact that the crystal lattice of the metal complexes is preserved afer irradiation with high intensity is unexpected, especially since computer simulation of the efect of fast neutrons on the same compound gives the
Scientific Reports | (2019) 9:13314 | https://doi.org/10.1038/s41598-019-49962-9 2 www.nature.com/scientificreports/ www.nature.com/scientificreports
Figure 2. Photoluminescent spectra of irradiated (red) and non-irradiated (blue) solid complexes [La(NpSON)3]2 (a) (excitation 395 nm), Eu(TTA)3(DME)2 (b) (excitation 370 nm) and THF solution of [Sm(OON)3]2 (c) (excitation 370 nm).
Figure 3. Molecular structure of the irradiated (grey) and non-irradiated (green) [Ce(OON)3]2 complex. Termal ellipsoids are drawn at 30% level probability. Hydrogen atoms are omitted for clarity.
opposite result. Calculations show that the efect of neutrons with energy of 500 keV on cerium atoms, as well as on other atoms, will cause their displacement by more than 100 nm from the initial position, i.e. should lead to the destruction of the substance (Fig. S2). Found contradiction experimental and calculated data is probably explained by the relatively low density of the applied neutron radiation: a fux was no more than 5·1013 n/cm2. Since the sample contained about 1·1019 Ce atoms, it is quite clear that even under the assumption that each neutron reaches the target, only an insignifcant part of the metal and other atoms undergoes an attack and this atoms are unable to exert a noticeable infuence on the overall structure of the complex and consequently on the optoelectronic properties of the substance. All the used compounds afer irradiation become radioactive due to the capture of thermal neutrons by atomic nuclei in the complexes. Magnitudes of the induced radioactivity in three days afer treatment (4.56, 6.29 and 4.52 μZ for La(NpSON)3, Sm(NpSON)3 and Eu(NpSON)3, respectively) indicate the formation of new isotopes of rare earth metals since radioactive isotopes of other elements in the complexes (C, O, S and
Scientific Reports | (2019) 9:13314 | https://doi.org/10.1038/s41598-019-49962-9 3 www.nature.com/scientificreports/ www.nature.com/scientificreports
N) have very short half-life and by the time of measurement the complexes contain only stable isotope of these element. As these data indicate nuclear reactions in metal-organic compounds, the question arises whether these reactions cause the destruction of the molecule of the complex or its structure remains unchanged? As it was showed by many previous studies, the nuclear reactions on the organometallic complexes as a rule lead to splitting of of the organic ligands and in some cases to a deep transformation of the latter16,17. Tis way is used for a preparation of new radioactive organometallic complexes18–20 in particular the complexes for neutron capture therapy21,22. In all these nuclear synthesis with organometallic compounds very few atoms (10−10%)16 undergo transformation. In our case, as shown by X-ray difraction studies of a cerium compound, the most of molecules in the lanthanide coordination complexes are not destroyed upon neutron bombardment of the material. Tis, obviously, explains their relatively high radiation stability and the preservation of the optoelec- tronic properties under the action of n,γ-irradiation. Methods Complexes of La, Ce, Nd, Sm, Eu, Tb and Yb with 2-(2-benzoxazol-2-yl)phenolate (OON)12 and 3-(2- benzoxazol-2-yl)-2-naphtholate (NpSON)13 ligands were synthesized as described earlier. Europium 2-thenoyltrifuoroacetonate Eu(TTA)3(DME)2 was synthesized under anaerobic conditions by the reaction of Eu[N(SiMe3)2]3 (67 mg, 0.106 mmol) with tris(4,4,4-trifuoro-1-(2-thienyl)-1,3-butanedione) (H(TTA)) (70 mg, 0.315 mmol) in DME (10 ml) at room temperature (10 min.) and isolated in the form of a light yellow powder. Yield 81 mg (76%). Anal. Calcd. (%) for C32H35EuF9O10S3 (998.76) C, 38.48; H, 3.53; Eu, 15.22; S, 9.63. Found (%) C, 38.46; H, 3.57; Eu, 15.26; S, 9.59. IR (KBr, ν, cm−1): 1623 (s), 1600 (s), 1577 (s), 1540 (s), 1511 (s), 1413 (s), 1395 (s), 1306 (s), 1256 (m), 1233 (m), 1187 (m), 1139 (s), 1056 (m), 1030 (m), 936 (m), 865 (m), 791 (s), 770 (w), 710 (m), 685 (m), 643 (s), 583 (s). Te C, H, N elemental analyses were performed by the Microanalytical laboratory of IOMC on Euro EA 3000 Elemental Analyser. Te lanthanides content was analyzed by complexometric titra- tion. IR spectra were obtained on a FTIR spectrometer FSM-1201 and recorded from 4000 to 400 cm–1 as a Nujol mull on KBr plates. Emission spectra were registered from 300 to 700 nm on a fuorescent spectrometer Perkin Elmer LS-55. Te prototypes of photovoltaic cells were designed and tested as described elsewhere23. Samples of the complexes (100–150 mg) in the form of a fne crystalline powder were placed in glass tubes with a diameter of 2.5 mm and a wall thickness of 1 mm. Te tubes were evacuated, sealed and treated with n,γ-irradiation for 45 h at a sustained mode. Te absorbed dose of radiation was 12 krad with a fux of neutrons of 6 ·1012 n/cm2. Te same samples were repeatedly treated for 45 hours with more intense radiation (absorbed 13 2 dose of 120 krad with a flux of 5·10 n/cm ). Samples of the complexes [La(NpSON)3]2, [Nd(NpSON)3]2, [Sm(NpSON)3]2, [Eu(NpSON)3]2 in the form of fne-crystalline powders and the cerium complex [Ce(OON)3]2 in the form of crystals, prepared as in previous experiments12, were irradiated with an pulse mode (duration of 3 ms). Absorbed dose was 130 krad at a fux of neutrons of 3.6·1013 n/cm2. Afer each irradiation, the IR spectrum was recorded for all compounds. For the compounds [Nd(NpSON)3]2, [Sm(OON)3]2 and Eu(TTA)3(DME)2 the photoluminescence spectra of solid samples and THF solutions were recorded. For the sample of the complex [Yb(NpSON)3]2, the photovoltaic characteristics were determined in the planar photovoltaic cell of confguration ITO/complex (25 nm)/C60 (40 nm)/Bphen (8 nm)/Al (Bphen – 4,7-diphenyl-1,10-phenanthroline) which was fab- ricated by vacuum evaporation method as described earlier24. In the case of the cerium complex [Ce(OON)3]2 afer irradiation, its molecular structure was studied by X-ray difraction method using a Bruker D8 Quest difractometer (MoKα radiation, ω-and ϕ-scan technique, λ = 0.71073 Å). The intensity data were integrated by SAINT program25. SADABS26 was used to perform area-detector scaling and absorption corrections. Te structure was solved by dual-space27 method and refned on F2 using all refections with the SHELXTL package28,29. All non-hydrogen atoms were refned anisotropically. H atoms were placed in calculated positions and refned in the “riding model”. Te details of crystallographic, collection and refnement data for [Ce(OON)3]2 are presented in Table S1 and S2. CCDC-1877840 contains the supplementary crystallographic data for this paper. Tese data can be obtained free of charge from the Cambridge Crystallographic Data Centre via www.ccdc.cam.ac.uk/data_request/cif. A mathematical model of the destruction of the cerium complex [Ce(OON)3]2 under the neutron irradiation was carried out by the Monte Carlo method using the SRIM-2003 sofware package30. Te calculation of the cross sections for the interaction of neutrons with atoms of the complexes was performed for average neutron energy of 2 MeV. Additional calculations were made for energy of 100 keV and 10 MeV. In the course of calculations, the neutron radiation energy was varied, and a trial calculation of the efect of gamma rays was also carried out. A comparison of the processes of defect formation in the studied materials was made for light and heavy atoms in a substance. Te trajectory of each recoil atom, which received energy upon the impact of a neutron, began with the input of its position, direction of motion, and energy. Over the free path length of the recoil atoms, their energy decreased by the amount of electronic losses for ionization of the material, and then, afer a collision, by so-called nuclear, or elastic energy losses, i.e. on the energy transferred to the target atom in a collision. Te energy trans- ferred by neutrons to recoil atoms and responsible for radiation violations was calculated by the formula (1)30
4MM θ 4A T = nA T sin2 = T a 2 nn 22 ()MMnA+ 2 (1 + A ) (1)
where Мn, МА is the mass of a neutron and an atom; Tn is the kinetic energy of a bombarding neuron; θ is the recoil angle between the direction of motion of the neutron before and afer the collision, A is the atomic weight. Te angle of scattering in the centre of mass system was defned as in the formula (2):
Scientific Reports | (2019) 9:13314 | https://doi.org/10.1038/s41598-019-49962-9 4 www.nature.com/scientificreports/ www.nature.com/scientificreports
Pp++δ cosθ= Tn pr+ 0 (2) Te selection of target atoms was made using random numbers. It was assumed that the probability of a colli- sion with an atom of each type is proportional to its stoichiometric coefcient determined by the brutto-formula. Te diference between light and heavy atoms in the target was the magnitude of the interaction potential. In the model of nonlocal energy loss, electron loss was determined as the multiplying of the braking function and the length of free path of the recoil atom. We used the Bragg rule, which states that the contribution to the stopping power of each type of target atoms is proportional to their atomic fraction. Conclusions Tus, with the example of organo-lanthanide complexes, the radiation resistance of molecular metal-organic compounds was studied for the frst time. It was found that the stability of the studied compounds with respect to the efects of n- and γ-radiation exceeds the stability of inorganic semiconductor materials. Study of the radiation resistance of organic compounds of lanthanides at the molecular level with the example of the cerium complex showed that the bombardment of the tested substances with fast neutrons with energy of ∼1 MeV and fax 5·1013 n/cm2 does not cause changes in the structure of most molecules, so the photophysical characteristics of the mate- rial are preserved. Te found high radiation resistance of organo-lanthanide complexes opens up the possibility of their use as functional materials in the design of devices and apparatus designed to work under conditions of enhanced radiation. References 1. Bunzli, J.-C. G. & Eliseeva, S. V. Lanthanide Luminescence Photophysical, Analytical and Biological Aspects (eds Hänninen, P. & Härmä, H.) 1–45 (Springer Verlag, 2011). 2. Stojanovic, N. M., Simic, B. B., Stankovic, K. D. J. & Lazarevic, D. R. Degradation efects of the output electrical characteristics of Si solar cells as a result of ionizing radiation under low light conditions. Nuclear Technology & Radiation Protection 30, 210–213 (2015). 3. Kawakita, S., Imaizumi, M., Ishizuka, S. & Shibata, H. & Okuda Shuichi Ionization efects on Cu(In, Ga)Se2 thin-flm solar cells. Phys. Status Solidi C, 1600168, https://doi.org/10.1002/pssc.201600168 (2017). 4. Lei, Y. et al. Te radiation damage of crystalline silicon PN diode in tritium beta-voltaic battery. Applied Radiation and Isotopes 90, 165–169 (2014). 5. Okuno, Y. et al. Radiation degradation prediction for InGaP solar cells by using appropriate estimation method for displacement threshold energy. Journal of Applied Physics 122, 114901–114907 (2017). 6. Tomas, A. K., Kouhestani, C. J. & Grey, J. K. Ionizing radiation exposure reveals instability of purifed domains in polymer/ fullerene solar cells. Solar Energy Materials & Solar Cells 160, 85–93 (2017). 7. Kouhestani, C. et al. Ionizing radiation induced parametric variations in P3HT:PCBM organic photovoltaic cells. Vacuum Science & Technology B 33, 032403–032406 (2015). 8. Doty, F. P., Bauer, C. A., Skulan, A. J., Grant, P. G. & Allendorf, M. D. Scintillating Metal‐Organic Frameworks: A New Class of Radiation Detection Materials. Adv. Mater. 21, 95–101 (2009). 9. Feng, P. L. et al. Designing metal-organic frameworks for radiation detection. Nucl. Instrum. Methods Phys. Res. Sect. A 652, 295–298 (2011). 10. Wang, C. et al. Synergistic Assembly of Heavy Metal Clusters and Luminescent Organic Bridging Ligands in Metal–Organic Frameworks for Highly Efcient X-ray Scintillation. J. Am. Chem. Soc. 136, 6171–6174 (2014). 11. Mathis, S. R. II et al. Mesoporous stilbene-based lanthanide metal organic frameworks: synthesis, photoluminescence and radioluminescence characteristics. Dalton Trans. 46, 491–500 (2017). 12. Balashova, T. V. et al. Lanthanide phenolates with heterocyclic substituents. Synthesis, structure and luminescent properties. Polyhedron 50, 112–120 (2013). 13. Burin, M. E. et al. Synthesis and luminescent properties of 3-(2-benzoxazol-2-yl)- and 3-(2-benzothiazol-2-yl)-2-naphtholates of some non-transition and rare earth metals. Synth. Met. 164, 55–59 (2013). 14. Pushkarev, A. P. et al. Lanthanide complexes with substituted naphtholate ligands: extraordinary bright near-infrared luminescence of ytterbium. Russ. Chem. Bull. 62, 392–397 (2013). 15. Katkova, M. A. et al. Near-infrared electroluminescent lanthanide [Pr(III), Nd(III), Ho(III), Er(III), Tm(III), and Yb(III)] N,O- chelated complexes for organic light-emitting devices. J. Mater. Chem. 21, 16611–16620 (2011). 16. Wiles, D. R. Te radiochemistry of organometallic compounds. Advances in Organometallic Chemistry 11C, 207–252 (1973). 17. Baumgartner, F. V. Untersuchungen über die Molekülneubildung bei der Neutroneneinfangreaktion. Radiochimica Acta 1, 51–55 (1963). 18. de Jong, I. G. & Wiles, D. R. Radiochemistry of organomolybdenum compounds. 2. Formation of technetium compounds by β− decay in η-cyclopentadienyltricarbonylmolybdenum. Inorg. Chem. 15, 2588–2591 (1976). 19. de Jong, I. G. & Wiles, D. R. Nuclear recoil reactions in organomanganese compounds. IV. Fulvalenehexacarbonyldimanganese. Can. J. Chem. 48, 1614–1615 (1970). 20. Campbell, K. S., Dillon, C. T., Smith, S. V. & Harding, M. M. Radiotracer studies of the antitumor metallocene molybdocene dichloride with biomolecules. Polyhedron 26, 456–459 (2007). 21. Salt, C., Lennox, A. J., Takagaki, M., Maguire, J. A. & Hosmaneа, N. S. Boron and Gadolinium Neutron Capture Terapy. Russ. Chem. Bull., Int. Ed. 53, 1871–1888 (2004). 22. De Stasio, G. P. et al. Gadolinium in human glioblastoma cells for gadolinium neutron capture therapy. Cancer Research 61, 4272–4277 (2001). 23. Maleev, A. A. et al. Photovoltaic properties of Zn, Al, La, Sm, and Yb complexes with o-iminobenzoquinone ligands. Nanotechnol. Russia 10, 613–620 (2015). 24. Maleev, A. A. et al. Monophthalocyanine complexes of samarium and terbium with axial ligands: synthesis, structure and optoelectronic properties. J. Rare Earths 32, 1101–1108 (2014). 25. SAINT. Data Reduction and Correction Program v. 8.37A, Bruker AXS, Madison, Wisconsin, USA, 2014. 26. SADABS. Bruker/Siemens Area Detector Absorption Correction Program, v. 2016/2, Bruker AXS, Madison, Wisconsin, USA. 27. Sheldrick, G. M. SHELXT - Integrated space-group and crystal-structure determination. Acta Cryst. A 71, 3–8 (2015). 28. Sheldrick, G. M. Crystal structure refnement with SHELXL. Acta Cryst. C 71, 3–8 (2015). 29. Krause, L., Herbst-Irmer, R., Sheldrick, G. M. & Stalke, D. Comparison of silver and molybdenum microfocus X-ray sources for single-crystal structure determination. J. Appl. Cryst. 48, 3–10 (2015). 30. Biersack, J. P. Computer simulations of sputtering. Nucl. Instrum. Methods Phys. Res., Sect. B 27, 21–36 (1987).
Scientific Reports | (2019) 9:13314 | https://doi.org/10.1038/s41598-019-49962-9 5 www.nature.com/scientificreports/ www.nature.com/scientificreports
Acknowledgements This work was supported by the Russian Science Foundation (Project № 18-13-00066). The synthesis of compounds was carried out with the support of the Russian Foundation for Basic Research (Grant No. 18-33- 00241). Te work was performed using the instrumental base of the Analytical Center of the G.A. Razuvaev Institute of Organometallic Chemistry, Russian Academy of Sciences. X-ray investigation was performed in the framework of the Russian state assignment (Temes № 45.6 and 44.2, Reg. № АААА-А19- 119011690055-0, АААА-А16-116122110053-1). Author Contributions T.V. Balashova – synthesis of the complexes studied. S.V. Obolensky – computer modeling. A.N. Trufanov – treatment of the samples with ionization irradiation. M.N. Ivin – treatment of the samples with ionization irradiation. V.A. Ilichev – measurement of IR and luminescence spectra. A.A. Kukinov – preparation of the samples for treatment with irradiation, design and test the photovoltaic cell. E.V. Baranov – X-ray analysis. G.K. Fukin – X-ray analysis. M.N. Bochkarev - statement of the problem, discussion of the results. All co-authors participated in the preparation of this article. Additional Information Supplementary information accompanies this paper at https://doi.org/10.1038/s41598-019-49962-9. Competing Interests: Te authors declare no competing interests. Publisher’s note Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional afliations. Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Cre- ative Commons license, and indicate if changes were made. Te images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not per- mitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
© Te Author(s) 2019
Scientific Reports | (2019) 9:13314 | https://doi.org/10.1038/s41598-019-49962-9 6